# Neural Network Model for Isothermal Pearlite ... · PDF file The isothermal...

date post

15-Oct-2020Category

## Documents

view

0download

0

Embed Size (px)

### Transcript of Neural Network Model for Isothermal Pearlite ... · PDF file The isothermal...

1

Neural Network Model for Isothermal Pearlite Transformation.

Part I: Interlamellar Spacing Model

C. CAPDEVILA, F. G. CABALLERO, and C. GARCÍA DE ANDRÉS

Dr. C. Capdevila and Dr. F. G. Caballero, Tenured Scientist, and Dr. C. García de Andrés,

Research Scientist, are in the Department of Physical Metallurgy, Centro Nacional de

Investigaciones Metalúrgicas (CENIM), CSIC, Avda. Gregorio del Amo, 8, 28040 Madrid,

Spain..

2

Abstract

The present paper is the first of a two-part paper which deals with a neural network model to

describe the isothermal pearlite formation. The isothermal austenite-to-pearlite transformation

has been analyzed using a neural network technique within a Bayesian framework. In this

framework, the pearlite interlamellar spacing and growth rate of pearlite can be represented as

a general empirical function of variables such as Mn, Cr, Ni, Si and Mo alloying contents and

temperature which are of great importance for the pearlite growth mechanisms. The method

has limitations owing to its empirical character, but it has been demonstrated that it can be

used in such way that the predicted trends make metallurgical sense. In this first part paper,

the method has been used to examine the relative importance of the alloying elements on

pearlite interlamellar spacing.

KEY WORDS: Neural Network Analysis; Pearlite; Interlamellar Spacing; Modelling Phase

Transformation; Steels

3

1. Introduction

Crude steel production by the major steel-producing countries is of the order of 850 millions

tones per annum, the vast majority of which is subsequently fabricated into plates, bars, rods,

strips, sheets and coils, using large scale deformation processes, in which the cooling rate

from austenite phase field is relatively slow. Such products are destined for use in the

construction, power generation, shipbuilding and automotive industries (among others), where

structural materials of high strength, good toughness, low cost and weldability are required.

The microstructure of these steels is usually a mixture of allotriomorphic ferrite and pearlite.

The mechanical properties are derived from these microstructural constituents.

Nowadays, there are available quantitative computerized models regarding ferrite and pearlite

transformation 1-6). Such models would yield information on composition, grain size and

distribution of phases and reaction kinetics, and the output of most of these models is the

evolution of volume fraction of phases. However, an intermediate stage of calculation is

necessary. More precisely, determination of interlamellar spacing is a key factor on the

austenite-to-pearlite transformation.

Interlamellar spacing is one of the most fundamental parameters that characterize the pearlite

microstructure. The wide range of mechanical properties of pearlitic microstructure, and

hence the main reason of why ferritic-pearlitic steels are by far the most consumed structural

material in the world, are intrinsically related to the pearlite interlamellar spacing. It is

therefore not surprising that it has been reported for decades the influence of alloying

elements and cooling conditions on interlamellar spacing of pearlite 7-8). On the other hand, it

has been recently reported the role of interlamellar spacing on austenite formation during the

isothermal and continuous heating austenite formation ,9). Thus, the study of the factors which

influence interlamellar spacing of pearlite formation is, at present, an interesting topic.

4

The purpose of the present work is to investigate whether an artificial neural network can be

trained to predict interlamellar spacing of pearlite and pearlite growth rate as a non-linear

function of chemical composition and temperature, and whether the patterns that emerge from

this model emulate the metallurgical experience.

In normal regression methods, the analysis begins with prior choice of a relationship (usually

linear) between the output and input variables. A neural network is capable of performing a

greater variety of non-linear relationships of considerable complexity. Data are presented to

the network in the form of input and output parameters, and the optimum non-linear

relationship is found by minimizing a penalized likelihood. In effect the network tries out

many kinds of relationships in its search for an optimum fit. As in regression analysis, the

results consist of a function that relates the inputs to the outputs by a series of coefficients

called weights. In spite of its apparent sophistication, the method is as blind as regression

analysis, and neural networks can be susceptible to overfitting. This paper deals with the

analysis of the influence of alloying elements such as Mn, Cr, Ni, Si, and Mo, separately and

together, on interlamellar spacing by means of neural networks.

2. Experimental: Build of the model

2.1. Technique

Neural networks are parameterized non-linear models used for empirical regression and

classification modeling. Their flexibility enables them to discover more complex relationships

between the data than traditional linear statistical models.

A neural network is ‘trained’ on a set of examples of input and output data. The outcome of

the training is a set of coefficients (referred to as weights) and a specification of the functions

which in combination with the weights relate the input to the output. The training process

5

involves a search for the optimum non-linear relationship between the input and output data

and is computer intensive. Once the network is trained, estimation of the outputs for any

given inputs is very rapid.

One of the difficulties with blind data modeling is that of ‘overfitting’, in which spurious

details and noise in the training data are overrated by the model. This gives rise to solutions

that generalize poorly. MacKay 10-11) has developed a Bayesian framework for neural

networks in which the appropriate model complexity is inferred from the data.

The Bayesian framework for neural networks has two further advantages. First, the

significance of the input variables is automatically quantified. Consequently, the significance

perceived by the model of each input variable can be compared against metallurgical theory.

Second, the network's predictions are accompanied by error bars which depend on the specific

position in input space. These quantify the model's certainty about its predictions.

2.2. The experimental database

Two measured parameters may characterize the interlamellar spacing of pearlite: the average

minimum observed spacing taken from several colonies, and the mean intercept spacing. The

former parameter is a perpendicular distance across two consecutives lamellae i.e. ferrite and

cementite, while the mean intercept spacing is an average distance across two successive

lamellae taken from test lines randomly applied to the plane of polish.

Experimental evidence in pearlite produced under isothermal conditions prove that the true

spacing is not the minimum spacing observed in metallographically prepared surfaces. The

true spacing does not have a constant value, but it is a distribution of spacings about a mean

true value. Stereological studies concluded that the mean true spacing of pearlite is half of the

mean intercept spacing 12). By contrast, the factor which relates the minimum and the mean

6

true spacing is not constant and may vary from system to system, and with transformation

temperature in a given system. It is because of the uncertainty in the relationship between the

minimum and the mean true spacing that the former parameter is sometimes reported as the

parameter that characterizes the pearlite microstructure. However, it would be in fact more

satisfactory to characterize the microstructure in terms of the mean true spacing (So). In this

sense, the interlamellar spacing parameter in the database corresponds to mean true spacings

reported in literature for eutectoid steels.

A complete description of the chemical composition and the isothermal transformation

temperature is required to ideally model the interlamellar spacing of pearlite in steels. A

search of the literature 5,7,13-18) allows us to collect 220 individual cases where detailed

chemical composition, isothermal temperature, and So values were reported. Table I shows

the list of 6 input variables used for the interlamellar spacing analysis.

(Table I)

2.3. Neural network analysis

The aim is to be able to estimate the pearlite interlamellar spacing as a function of the input

variables listed in Table I. The network consists of 6 input nodes, a number of hidden nodes,

and an output node representing the interlamellar spacing of pearlite (Fig. 1). The network

was trained using 110 examples randomly chosen from a total of 220 available, the remaining

110 examples being used as ‘new’ experim